formation of hierarchically organized zeolites by sequential ......zeolites doi:...
Embed Size (px)
Formation of Hierarchically Organized Zeolites by SequentialIntergrowth**Watcharop Chaikittisilp, Yuki Suzuki, Rino R. Mukti, Tatsuya Suzuki, Keisuke Sugita,Keiji Itabashi, Atsushi Shimojima, and Tatsuya Okubo*
Hierarchically organized porous materials can provide multi-dimensional spatial networks on different length scales withimproved characteristics relevant to molecular diffusion.
Zeolites that are microporous crystalline materials havingpores and channels at molecular dimensions are of greatimportance for industrial applications. However, the pres-ence of only micropores in zeolite frameworks often limits themolecular diffusion and therefore, restricts the transport ofbulky molecules. This problem can be resolved by shorteningthe effective diffusion path lengths, which has been achievedby miniaturizing zeolite crystals, delaminating or exfoliatinglayered zeolites, synthesizing zeolite nanosheets, andintroducing mesopores into zeolite particles.[6–12] Amongthese solutions, the fabrication of hierarchical zeolites withmicro- and mesoporosity is of interest because it combinesintrinsic micropores with bypass-interconnected mesopores,and therefore, enhances both the micropore accessibility andmolecular traffic within zeolite particles.[1,7b, 12]
Hierarchical zeolites have been produced using severaltechniques, including top-down desilication by alkali post-synthetic treatment and bottom-up directed assembly byhard or soft[8–11] templates. The hard-template methodrequires multistep procedures and is therefore unfavorablefor large-scale production. Alternatively, the direct introduc-tion of organic mesopore-generating agents (mesoporogens)during zeolite synthesis can create uniform mesopores. Theuse of such mesoporogens is currently one of the mostpromising methods for the single-step construction of hier-archical zeolites. Progress has been made using well-designedmesoporogens composed of long hydrophobic chains andhydrophilic zeolitic structure-directing groups to generate
zeolites with tunable mesoporosity[9a, 10] and to direct thehierarchical assembly of zeolite nanosheets, yielding meso-porous zeolites with house-of-cards-like structures.[5a, 9c,11]
These hierarchical nanosheets showed excellent catalyticperformance in several important reactions because thepresence of thin layers with specific crystalline faces facili-tates catalysis at the exteriors or pore mouths. Suchmesoporogens are probably necessary for the direct, single-step synthesis of hierarchical zeolites.
Herein we report an alternative, mesoporogen-freeapproach for the construction of hierarchically organizedMFI zeolites by sequential intergrowth using a simple organicstructure-directing agent (OSDA). The selection of anappropriate OSDA and optimized synthesis conditions thatcan form plate-like zeolites with enhanced 908 rotationalintergrowths seems to be a key to achieving a hierarchicalstructure with three classes of porosity in one structure: theintrinsic microporosity of the zeolite framework together withmesoporosity existing within the zeolite plates and macro-porosity stemming from the complex intergrown structure.
Epitaxial and rotational intergrowths are commonlyobserved in many zeolites. We have hypothesized that byengineering the zeolite intergrowths, hierarchically organizedzeolites can be constructed without the need for mesopor-ogens. In particular, we have focused on the MFI zeolitebecause it is an excellent catalyst in many industrial proc-esses[2b,15] and a promising material for membrane separa-tion.[1b] MFI zeolite that contains sinusoidal channels alongthe a axis interconnected with straight channels along the baxis is often formed with 908 rotational intergrowths, in whichsubstantial (h00) faces are epitaxially overgrown on the (0k0)
[*] Dr. W. Chaikittisilp,[$] [+] Y. Suzuki,[#] [+] Dr. R. R. Mukti,[++]
Dr. K. Itabashi, Prof. Dr. A. Shimojima, Prof. Dr. T. OkuboDepartment of Chemical System EngineeringThe University of Tokyo7-3-1 Hongo, Bunkyo-ku, Tokyo 113-8656 (Japan)E-mail: [email protected]: http://www.zeolite.t.u-tokyo.ac.jp
Dr. T. Suzuki, Dr. K. SugitaBasic Chemicals Research LaboratorySumitomo Chemical Co. Ltd.5-1 Sobiraki-cho, Niihama, Ehime 792-8521 (Japan)
[++] Present address: Division of Inorganic and Physical Chemistry,Institut Teknologi BandungJl. Ganesha no. 10, Bandung 40132 (Indonesia)
[$] Present address: World Premier International (WPI) ResearchCenter for Materials Nanoarchitectonics (MANA),National Institute for Materials Science1-1 Namiki, Tsukuba, Ibaraki 305-0044 (Japan)
[#] Present address: Technical Research & Development BureauNippon Steel & Sumitomo Metal Corporation20-1 Shintomi, Futtsu, Chiba 293-8511 (Japan)
[+] These authors contributed equally to this work.
[**] This study was supported in part by Sumitomo Chemical Co. Ltd.,a Grant-in-Aid for Scientific Research (B) from the Japan Society forthe Promotion of Science (JSPS), and a Global COE Program(Mechanical Systems Innovation) from the Ministry of Education,Culture, Sports, Science and Technology (MEXT) (Japan). W.C.thanks MEXT for a Monbukagakusho Scholarship. R.R.M. thanksJSPS for a postdoctoral fellowship. We are grateful to Dr. YoshihiroKamimura for his assistance with the solid-state NMR measure-ments.
Supporting information for this article is available on the WWWunder http://dx.doi.org/10.1002/anie.201209638.
3355Angew. Chem. Int. Ed. 2013, 52, 3355 –3359 � 2013 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
faces.[14a,16] The tetrapropylammonium (TPA) cation is themost common and probably the most energetically favoredOSDA for MFI zeolite formation. TPA cations are situatedat the intersection of the straight and sinusoidal channels.Therefore, we have considered that organic molecules withslight differences from TPA molecules could still direct thecrystallization of MFI zeolites but could also enhance theformation of 908 rotational intergrowths. Very recently, ina similar strategy, self-pillared zeolite nanosheets containingmicro- and mesoporosity were synthesized by repetitivebranching using tetrabutylphosphonium cations as anOSDA. Although the hierarchical zeolites could beobtained without the use of mesoporogens, the use ofa phosphonium-based OSDA would affect the physicochem-ical properties of the resultant zeolites because the decom-position of the OSDA by conventional thermal calcinationcannot totally remove phosphorus from the zeolite structure,and therefore, a certain amount of phosphorus debris mayremain in the zeolites.
Among the many OSDAs for MFI zeolite, we havefocused herein on dimers of the TPA cation, (C3H7)3N
+(C3H7)3, because such diquaternary ammoniumcations with n = 5–7 are situated in the framework with theN-N chains being better fitted along the straight channelsthan along the sinusoidal channels. This limits the degree ofmolecular motion within the framework, particularly in thecase of OSDAs with shorter alkyl-chain spacers. The TPAdimer with n = 5, hereafter denoted as diquat-C5, possessesan intramolecular N-N distance of 0.7 nm, which is muchshorter than the distances between two intersections along thestraight (1.0 nm) and sinusoidal (1.2 nm) channels. Althoughprevious molecular mechanics simulations suggested thatdiquat-C5 is not readily accommodated in the zeolitechannels, it can still direct the formation of MFI zeolites.[18a,c]
Accordingly, the diquat-C5 cations have to adapt theirintramolecular N-N distance to be occluded intact withinthe MFI framework, perhaps along the straight channel,generating structural constraints or stresses, and therebyyielding framework distortion, as suggested by synchrotronX-ray analyses.[18c] This event limits crystal growth along the baxis, resulting in an MFI zeolite with a plate-like morphologybut with a few intergrowths.[18c] To generate hierarchicalzeolites composed of such plate-like crystals, zeolites shouldbe synthesized under conditions with more pronouncedsurface nucleation. In a previous report,[18c] zeolites weresynthesized from very dilute solutions in the presence of seedcrystals, thus limiting the formation of intergrowths. Althougha non-seeded synthesis was also carried out, the formation ofintergrowths was inhibited because the diquat-C5 partiallydecomposed under the synthetic conditions.
Field-emission scanning electron microscopy (FE-SEM)and secondary electron (SE) images of the product obtainedafter hydrothermal synthesis at 130 8C for 264 hours areshown in Figure 1 a,b, respectively (see experimental detailsin the Supporting Information). The powder X-ray diffraction(XRD) pattern (Figure 2a) confirms that the obtainedproduct possesses the MFI zeolite structure. These siliceousMFI (silicalite-1) zeolite crystals have an unusual intergrownorganization because of the 908 rotation of the adjoining
faces. To the best of our knowledge, this is the firstobservation of such a complex morphology for an MFIzeolite. The bright-field scanning transmission electron mi-croscopy (BF-STEM) images reveal that the zeolite plates areprobably constructed by the aggregation of nanoparticles(Figure 1c,d). The dot patterns of selected-area electrondiffraction (SAED) of both the main plate (Figure 1e) andthe crystal flake (Figure 1 f) indicate single-crystalline mate-rials. In addition, both SAED patterns reveal that the crystalsare viewed along the  zone axis, suggesting that the b axis(i.e., the straight channels) runs perpendicular to the surfaceof each crystal plate.
To obtain further insights into the organization process,the textural evolution of the obtained silicalite-1 crystals wasinvestigated, as shown in Figure 2. The first visible Braggdiffraction appears after 135 hours of crystallization (seeFigure 2a). Before the onset of crystallization, the FE-SEMimage shows that the products are nanoparticle aggregates(Figure 2b). No crystal-like, faceted particles were observedat this stage, consistent with the corresponding XRD pattern.After 135 hours (Figure 2c), the plate-like particles were firstseen together with the nanoparticle aggregates. These plate-like particles were probably silicalite-1 crystals, as suggested
Figure 1. a) FE-SEM, b) SE, c,d) BF-STEM, and e,f) TEM images ofsilicalite-1 zeolites synthesized at 130 8C for 264 h. The rough back-ground in (a) is carbon paste used for sample preparation. The squarearea in (c) is shown as a magnified image in (d). Insets in (e,f) areSAED patterns taken from the circled regions in the correspondingTEM images.
3356 www.angewandte.org � 2013 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim Angew. Chem. Int. Ed. 2013, 52, 3355 –3359
by the XRD pattern. The unusual intergrown structuredeveloped gradually during the course of crystallization(Figure 2d,e).
The calcined products synthesized at 130 8C for 150 hourswere further characterized by TEM. The SAED patterns ofrepresentative regions of the nanoparticle aggregates areshown in the insets of Figure 3 a and Figure S1 a, confirmingthat the resulting nanoparticles are amorphous. High-reso-lution TEM (HR-TEM) images (Figure 3b; Figure S1b)further supported the amorphous nature of these nano-particles. As expected, in contrast, plate-like particles exhib-ited SAED patterns common to MFI zeolite (Figure 3c;
Figure S1c; insets). Lattice fringesindicative of crystalline orders wereclearly observed in the HR-TEMimages (Figure 3d; Figure S1 d), cor-roborating that the plate-like particlesare silicalite-1 zeolites.
A scheme of the formation ofhierarchically organized MFI zeolitesbased on the above results is shown inFigure 4. In the early stage of crystal-lization, the amorphous nanoparticles,probably hydrated diquat-C5-silicacomposites, are formed. These compo-site nanoparticles aggregate to formvery thin MFI zeolite plates. Althoughthe formation process is still unclear,viable zeolite nuclei may be formed bythe oriented-aggregation mechanism,the solid-state-like disorder-to-ordertransformation, reorganization at thesolid-liquid interface, or a combinationthereof. Under the present synthesisconditions, the 908 rotational inter-
growths are enhanced and developed during the crystalgrowth process. The intergrown crystal flakes are also made ofnanoparticle aggregates. The composite nanoparticles and thesoluble species together supply the precursors for crystalgrowth, and subsequently, zeolite crystals evolve into thehierarchical structure.
We considered that increasing the synthesis temperaturecould enhance the crystal intergrowth, thereby enhancingthe formation of the hierarchical structures. Therefore,silicalite-1 zeolites were also synthesized at 150 8C and175 8C. Clearly, the hierarchical structure is more pronouncedafter synthesis at 150 8C, as shown in Figure 5a–c. The powder
Figure 2. a) Powder XRD patterns of the products obtained at 130 8C after 120–264 h. FE-SEMimages of the products after reaction times of b) 120 h, c) 135 h, d) 150 h, and e) 184 h.
Figure 3. a,c) TEM and b,d) HR-TEM images of the calcined productssynthesized at 130 8C for 150 h. HR-TEM images in (b,d) correspondto those in (a,c), respectively. Insets in (a,c) show the correspondingSAED patterns taken from the circled areas.
Figure 4. Schematic representation of the formation of hierarchicallyorganized MFI zeolite. a) Amorphous nanoparticles, probably hydrateddiquat-C5–silica composites, form from a solution. These nanoparti-cles aggregate to form MFI zeolite plates. b) The 908 rotationalintergrowths develop during crystal growth, in which each intergrowncrystal flask also forms from nanoparticle aggregates. c) The nano-particles and the soluble species in solution together supply theprecursors for crystal growth, and finally, zeolite crystals evolve intothe hierarchical structure.
3357Angew. Chem. Int. Ed. 2013, 52, 3355 –3359 � 2013 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim www.angewandte.org
XRD patterns (Figure 5 d) confirmed that the products areMFI zeolite. Interestingly, plate-like silicalite-1 zeolites withless-intergrown structures were obtained when the synthesistemperature was further raised to 175 8C (Figure S2). Wespeculate that Ostwald�s law of successive reactions is, at leastin part, responsible for the formation of the less-intergrownsilicalite-1 at 175 8C. This law essentially describes theconsumption of the less-stable phase, the subsequent forma-tion of a thermodynamically more stable phase, and so on,until the most stable phase is formed. At 175 8C, suchsuccessive ripening proceeds rapidly, and therefore, theresulting zeolites did not form the hierarchical structure.Observation of such less-intergrown silicalite-1 synthesized at130 8C and 150 8C after prolonged reaction times (Figure S3)additionally supported the theory of Ostwald ripening. Theseresults also suggest that the obtained silicalite-1 was the resultof a kinetically controlled synthetic pathway.
As is well known, quaternary ammonium cations canundergo a Hofmann elimination, particularly at high temper-ature. The solid-state 1H-13C cross-polarization magic-anglespinning (CP/MAS) NMR spectrum of the silicalite-1 synthe-sized at 150 8C reveals that the diquat-C5 cations are occludedintact in the zeolite product (Figure S4). In contrast, theproduct synthesized at 175 8C showed additional signals,
probably arising from Hofmann elimination products. Forexample, the signals at d� 30, 118, and 137 ppm can beassigned to the center carbon of 1,4-pentadiene, the b-olefiniccarbon (CH2CH=CH2), and the a-olefinic carbon (CH2CH=CH2), respectively. This partial decomposition of the diquat-C5 SDA seems to affect the morphology of the resultingzeolite products,[18b,c] in addition to Ostwald�s ripening.
Nitrogen sorption isotherms of the silicalite-1 sampleshow a large uptake at low relative pressures, a hysteresis loopat moderate relative pressures, and a slight uptake at higherrelative pressures, indicating the presence of micro-, meso-,and macroporosity, respectively (Figure 5e). The apparentspecific Brunauer–Emmett–Teller (BET) surface area andthe total pore volume (at P/Po = 0.99) were calculated to be490 m2 g�1 and 0.35 cm3 g�1, respectively. The external surfacearea and micropore volume were estimated by the t-plotmethod to be 215 m2 g�1 and 0.11 cm3 g�1, respectively. Thepore-size distribution and cumulative pore volume calculatedby non-local density functional theory (NL-DFT) aredepicted in Figure 5 f. The pore-size distribution was rela-tively narrow with a diameter centered at 3.3 nm. The SEM,TEM, and nitrogen physisorption results indicate that thesilicalite-1 zeolite possessed the intrinsic microporosity ofa zeolite framework together with mesoporosity within thezeolite plates and macroporosity stemming from the complexintergrown structure.
We also explored the synthesis of aluminosilicate MFI(ZSM-5) by adding an aluminum source to the startingsynthesis solution at different Si/Al ratios. The powder XRDpatterns confirmed the formation of MFI zeolite (Fig-ure S5a). The obtained ZSM-5 zeolites showed a similarmorphology, indicating that the presence of Al did not inhibitthe formation of this unique structure (Figure S5 c,d). Solid-state 27Al MAS NMR spectra of the calcined samples(Figure S5 b) suggested that Al atoms are located at thetetrahedral positions of the framework, although non-frame-work, octahedral Al species also appear. The nitrogensorption isotherms in Figure S6 a show that the obtainedZSM-5 also possesses micro-, meso-, and macroporosity. NL-DFT analyses confirmed the presence of mesoporosity (Fig-ure S6b), although the mesopore size distributions were lessuniform than that of the silicalite-1 counterpart (see above).These hierarchical ZSM-5 zeolites are potentially promisingfor the catalytic conversion of bulky molecules and biomassprocessing. Such topics are vital and merit a detailed inves-tigation in future studies.
In summary, we have demonstrated a new approach forthe construction of hierarchically organized zeolites bysequential intergrowth. For the first time, a complex andunusual morphology was observed for MFI zeolites. Thesezeolites possessing micro-, meso-, and macroporosity havebeen produced by a simple, single-step, hydrothermal syn-thesis using a small OSDA without meso- or macroporogens.The use of an OSDA that is imperfectly fitted to the zeoliteframework, yet can direct its formation, is thought to beresponsible for the formation of very thin zeolite plates withenhanced 908 rotational intergrowth, thereby for the con-struction of hierarchically organized structure. This conceptwould be applicable to other zeolite frameworks and related
Figure 5. a–c) FE-SEM images of the products obtained after crystal-lization at 150 8C for 216 h. d) Powder XRD patterns of the productsobtained after 120–216 h. e) Nitrogen adsorption (*)-desorption (*)isotherms and f) corresponding NL-DFT pore size distribution andcumulative pore volume of the calcined product after crystallization for216 h.
3358 www.angewandte.org � 2013 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim Angew. Chem. Int. Ed. 2013, 52, 3355 –3359
porous crystalline materials that can form such rotationalintergrowths.
Received: December 2, 2012Published online: February 18, 2013
.Keywords: crystal growth · hierarchical organization ·mesoporous materials · structure-directing agents · zeolites
 a) M. Hartmann, Angew. Chem. 2004, 116, 6004 – 6006; Angew.Chem. Int. Ed. 2004, 43, 5880 – 5882; b) M. A. Snyder, M.Tsapatsis, Angew. Chem. 2007, 119, 7704 – 7717; Angew. Chem.Int. Ed. 2007, 46, 7560 – 7573; c) J. P�rez-Ram�rez, C. H.Christensen, K. Egeblad, C. H. Christensen, J. C. Groen,Chem. Soc. Rev. 2008, 37, 2530 – 2542.
 a) M. E. Davis, Nature 2002, 417, 813 – 821; b) A. Corma, Chem.Rev. 1997, 97, 2373 – 2420.
 L. Tosheva, V. P. Valtchev, Chem. Mater. 2005, 17, 2494 – 2513. a) A. Corma, V. Fornes, S. B. Pergher, Th. L. M. Maesen, J. G.
Buglass, Nature 1998, 396, 353 – 356; b) S. Maheshwari, E.Jordan, S. Kumar, F. S. Bates, R. L. Penn, D. F. Shantz, M.Tsapatsis, J. Am. Chem. Soc. 2008, 130, 1507 – 1516.
 a) M. Choi, K. Na, J. Kim, Y. Sakamoto, O. Terasaki, R. Ryoo,Nature 2009, 461, 246 – 249; b) W. Park, D. Yu, K. Na, K. E. Jelfs,B. Slater, Y. Sakamoto, R. Ryoo, Chem. Mater. 2011, 23, 5131 –5137.
 a) M. Ogura, Catal. Surv. Asia 2008, 12, 16 – 27; b) M. Ogura, S.Shinomiya, J. Tateno, Y. Nara, E. Kikuchi, M. Matsukata, Chem.Lett. 2000, 882 – 883; c) J. C. Groen, L. A. A. Peffer, J. A.Moulijn, J. P�rez-Ram�rez, Chem. Eur. J. 2005, 11, 4983 – 4994;d) D. Verboekend, S. Mitchell, M. Milina, J. C. Groen, J. P�rez-Ram�rez, J. Phys. Chem. C 2011, 115, 14193 – 14203.
 a) W. Fan, M. A. Snyder, S. Kumar, P.-S. Lee, W. C. Yoo, A. V.McCormick, R. L. Penn, A. Stein, M. Tsapatsis, Nat. Mater. 2008,7, 984 – 991; b) H. Chen, J. Wydra, X. Zhang, P.-S. Lee, Z. Wang,W. Fan, M. Tsapatsis, J. Am. Chem. Soc. 2011, 133, 12390 – 12393;c) S.-S. Kim, J. Shah, T. J. Pinnavaia, Chem. Mater. 2003, 15,1664 – 1668.
 a) F.-S. Xiao, L. Wang, C. Yin, K. Lin, Y. Di, J. Li, R. Xu, D. S. Su,R. Schlçgl, T. Yokoi, T. Tatsumi, Angew. Chem. 2006, 118, 3162 –3165; Angew. Chem. Int. Ed. 2006, 45, 3090 – 3093; b) H. Wang,T. J. Pinnavaia, Angew. Chem. 2006, 118, 7765 – 7768; Angew.Chem. Int. Ed. 2006, 45, 7603 – 7606.
 a) M. Choi, H. S. Cho, R. Srivastava, C. Venkatesan, D.-H. Choi,R. Ryoo, Nat. Mater. 2006, 5, 718 – 723; b) K. Na, M. Choi, W.Park, Y. Sakamoto, O. Terasaki, R. Ryoo, J. Am. Chem. Soc.2010, 132, 4169 – 4177; c) K. Na, W. Park, Y. Seo, R. Ryoo, Chem.Mater. 2011, 23, 1273 – 1279.
 R. R. Mukti, H. Hirahara, A. Sugawara, A. Shimojima, T.Okubo, Langmuir 2010, 26, 2731 – 2735.
 A. Inayat, I. Knoke, E. Spiecker, W. Schwieger, Angew. Chem.2012, 124, 1998 – 2002; Angew. Chem. Int. Ed. 2012, 51, 1962 –1965.
 X. Zhang, D. Liu, D. Xu, S. Asahina, K. A. Cychosz, K. V.Agrawal, Y. A. Wahedi, A. Bhan, S. A. Hashimi, O. Terasaki, M.Thommes, M. Tsapatsis, Science 2012, 336, 1684 – 1687.
 A. Corma, Nature 2009, 461, 182 – 183. a) E. Stavitski, M. R. Drury, D. A. M. de Winter, M. H. F. Kox,
B. M. Weckhuysen, Angew. Chem. 2008, 120, 5719 – 5722;Angew. Chem. Int. Ed. 2008, 47, 5637 – 5640; b) J. M. Newsam,M. M. J. Treacy, W. T. Koetsier, C. B. de Gruyter, Proc. R. Soc.London Ser. A 1988, 420, 375 – 405; c) G. R. Millward, S.Ramdas, J. M. Thomas, M. T. Barlow, J. Chem. Soc. FaradayTrans. 2 1983, 79, 1075 – 1082; d) M. M. J. Treacy, D. E. W.Vaughan, K. G. Strohmaier, J. M. Newsam, Proc. R. Soc.London Ser. A 1996, 452, 813 – 840; e) T. Okubo, T. Wakihara,J. Pl�vert, S. Nair, M. Tsapatsis, Y. Ogawa, H. Komiyama, M.Yoshimura, M. E. Davis, Angew. Chem. 2001, 113, 1103 – 1105;Angew. Chem. Int. Ed. 2001, 40, 1069 – 1071; f) T. Wakihara, S.Yamakita, K. Iezumi, T. Okubo, J. Am. Chem. Soc. 2003, 125,12388 – 12389.
 Y. Izumi, H. Ichihashi, Y. Shimazu, M. Kitamura, H. Sato, Bull.Chem. Soc. Jpn. 2007, 80, 1280 – 1287.
 a) T. Nakazawa, M. Sadakata, T. Okubo, Microporous Meso-porous Mater. 1998, 21, 325 – 332; b) W. Chaikittisilp, M. E.Davis, T. Okubo, Chem. Mater. 2007, 19, 4120 – 4122.
 M. E. Davis, R. F. Lobo, Chem. Mater. 1992, 4, 756 – 768. a) E. de Vos Burchart, J. C. Jansen, B. van de Graaf, H. van
Bekkum, Zeolites 1993, 13, 216 – 221; b) L. W. Beck, M. E. Davis,Microporous Mesoporous Mater. 1998, 22, 107 – 114; c) G.Bonilla, I. D�az, M. Tsapatsis, H.-K. Jeong, Y. Lee, D. G.Vlachos, Chem. Mater. 2004, 16, 5697 – 5705.
 a) T. M. Davis, T. O. Drews, H. Ramanan, C. He, J. Dong, H.Schnablegger, M. A. Katsoulakis, E. Kokkoli, A. V. McCormick,R. L. Penn, M. Tsapatsis, Nat. Mater. 2006, 5, 400 – 408; b) W.Fan, M. Ogura, G. Sankar, T. Okubo, Chem. Mater. 2007, 19,1906 – 1917; c) V. P. Valtchev, K. N. Bozhilov, J. Am. Chem. Soc.2005, 127, 16171 – 16177.